DOI: 10.17188/1308988
title: Materials Data on Li9Mn7V12O48 by Materials Project

description: Li9V12Mn7O48 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are nine inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with six VO4 tetrahedra and faces with two equivalent MnO6 octahedra. There are a spread of Li–O bond distances ranging from 2.00–2.12 Å. In the second Li1+ site, Li1+ is bonded to six O2- atoms to form distorted LiO6 octahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one LiO6 pentagonal pyramid, corners with six VO4 tetrahedra, and edges with two equivalent MnO6 octahedra. The corner-sharing octahedral tilt angles are 58°. There are a spread of Li–O bond distances ranging from 1.96–2.34 Å. In the third Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share a cornercorner with one LiO6 octahedra, a cornercorner with one MnO6 pentagonal pyramid, corners with six VO4 tetrahedra, and edges with two equivalent MnO6 octahedra. The corner-sharing octahedral tilt angles are 64°. There are a spread of Li–O bond distances ranging from 2.05–2.22 Å. In the fourth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share a cornercorner with one LiO6 octahedra, a cornercorner with one MnO6 pentagonal pyramid, corners with six VO4 tetrahedra, and edges with two equivalent MnO6 octahedra. The corner-sharing octahedral tilt angles are 64°. There are a spread of Li–O bond distances ranging from 2.04–2.22 Å. In the fifth Li1+ site, Li1+ is bonded to six O2- atoms to form distorted LiO6 pentagonal pyramids that share a cornercorner with one LiO6 octahedra, a cornercorner with one MnO6 octahedra, corners with six VO4 tetrahedra, and edges with two equivalent LiO6 pentagonal pyramids. The corner-sharing octahedra tilt angles range from 61–71°. There are a spread of Li–O bond distances ranging from 2.04–2.27 Å. In the sixth Li1+ site, Li1+ is bonded to six O2- atoms to form distorted LiO6 pentagonal pyramids that share a cornercorner with one LiO6 octahedra, a cornercorner with one MnO6 octahedra, corners with six VO4 tetrahedra, and edges with two equivalent MnO6 pentagonal pyramids. The corner-sharing octahedra tilt angles range from 63–71°. There are a spread of Li–O bond distances ranging from 2.02–2.33 Å. In the seventh Li1+ site, Li1+ is bonded to six O2- atoms to form distorted LiO6 octahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one LiO6 pentagonal pyramid, corners with six VO4 tetrahedra, and edges with two equivalent MnO6 octahedra. The corner-sharing octahedral tilt angles are 56°. There are a spread of Li–O bond distances ranging from 1.99–2.32 Å. In the eighth Li1+ site, Li1+ is bonded to six O2- atoms to form distorted LiO6 pentagonal pyramids that share corners with two MnO6 octahedra, corners with six VO4 tetrahedra, and edges with two equivalent LiO6 pentagonal pyramids. The corner-sharing octahedra tilt angles range from 58–59°. There are a spread of Li–O bond distances ranging from 2.12–2.22 Å. In the ninth Li1+ site, Li1+ is bonded to six O2- atoms to form LiO6 octahedra that share corners with six VO4 tetrahedra and faces with two equivalent MnO6 octahedra. There are a spread of Li–O bond distances ranging from 2.00–2.12 Å. There are twelve inequivalent V5+ sites. In the first V5+ site, V5+ is bonded to four O2- atoms to form VO4 tetrahedra that share corners with four LiO6 octahedra and corners with four MnO6 octahedra. The corner-sharing octahedra tilt angles range from 30–68°. There are a spread of V–O bond distances ranging from 1.73–1.80 Å. In the second V5+ site, V5+ is bonded to four O2- atoms to form VO4 tetrahedra that share corners with two LiO6 octahedra, corners with three MnO6 octahedra, and corners with three LiO6 pentagonal pyramids. The corner-sharing octahedra tilt angles range from 34–65°. There are a spread of V–O bond distances ranging from 1.65–1.83 Å. In the third V5+ site, V5+ is bonded to four O2- atoms to form VO4 tetrahedra that share corners with two LiO6 octahedra, corners with three MnO6 octahedra, and corners with three LiO6 pentagonal pyramids. The corner-sharing octahedra tilt angles range from 35–64°. There are a spread of V–O bond distances ranging from 1.64–1.83 Å. In the fourth V5+ site, V5+ is bonded to four O2- atoms to form VO4 tetrahedra that share corners with two LiO6 octahedra, corners with three MnO6 octahedra, a cornercorner with one MnO6 pentagonal pyramid, and corners with two equivalent LiO6 pentagonal pyramids. The corner-sharing octahedra tilt angles range from 25–63°. There are a spread of V–O bond distances ranging from 1.72–1.77 Å. In the fifth V5+ site, V5+ is bonded to four O2- atoms to form VO4 tetrahedra that share corners with two MnO6 octahedra, corners with three LiO6 octahedra, a cornercorner with one MnO6 pentagonal pyramid, and corners with two equivalent LiO6 pentagonal pyramids. The corner-sharing octahedra tilt angles range from 26–57°. There are a spread of V–O bond distances ranging from 1.68–1.79 Å. In the sixth V5+ site, V5+ is bonded to four O2- atoms to form VO4 tetrahedra that share corners with three LiO6 octahedra and corners with five MnO6 octahedra. The corner-sharing octahedra tilt angles range from 22–64°. There is three shorter (1.74 Å) and one longer (1.87 Å) V–O bond length. In the seventh V5+ site, V5+ is bonded to four O2- atoms to form VO4 tetrahedra that share corners with three MnO6 octahedra and corners with five LiO6 octahedra. The corner-sharing octahedra tilt angles range from 22–59°. There are a spread of V–O bond distances ranging from 1.68–1.81 Å. In the eighth V5+ site, V5+ is bonded to four O2- atoms to form VO4 tetrahedra that share corners with two MnO6 octahedra, corners with three LiO6 octahedra, and corners with three LiO6 pentagonal pyramids. The corner-sharing octahedra tilt angles range from 25–58°. There are a spread of V–O bond distances ranging from 1.68–1.85 Å. In the ninth V5+ site, V5+ is bonded to four O2- atoms to form VO4 tetrahedra that share corners with two LiO6 octahedra, corners with three MnO6 octahedra, and corners with three LiO6 pentagonal pyramids. The corner-sharing octahedra tilt angles range from 24–63°. There are a spread of V–O bond distances ranging from 1.65–1.81 Å. In the tenth V5+ site, V5+ is bonded to four O2- atoms to form VO4 tetrahedra that share corners with two MnO6 octahedra, corners with three LiO6 octahedra, a cornercorner with one LiO6 pentagonal pyramid, and corners with two equivalent MnO6 pentagonal pyramids. The corner-sharing octahedra tilt angles range from 33–59°. There are a spread of V–O bond distances ranging from 1.69–1.78 Å. In the eleventh V5+ site, V5+ is bonded to four O2- atoms to form VO4 tetrahedra that share corners with two MnO6 octahedra, corners with three LiO6 octahedra, a cornercorner with one LiO6 pentagonal pyramid, and corners with two equivalent MnO6 pentagonal pyramids. The corner-sharing octahedra tilt angles range from 34–59°. There are a spread of V–O bond distances ranging from 1.68–1.78 Å. In the twelfth V5+ site, V5+ is bonded to four O2- atoms to form VO4 tetrahedra that share corners with four LiO6 octahedra and corners with four MnO6 octahedra. The corner-sharing octahedra tilt angles range from 31–67°. There are a spread of V–O bond distances ranging from 1.72–1.79 Å. There are seven inequivalent Mn+3.86+ sites. In the first Mn+3.86+ site, Mn+3.86+ is bonded to six O2- atoms to form distorted MnO6 pentagonal pyramids that share corners with two LiO6 octahedra, corners with six VO4 tetrahedra, and edges with two equivalent LiO6 pentagonal pyramids. The corner-sharing octahedral tilt angles are 61°. There are a spread of Mn–O bond distances ranging from 1.93–2.25 Å. In the second Mn+3.86+ site, Mn+3.86+ is bonded to six O2- atoms to form MnO6 octahedra that share a cornercorner with one LiO6 octahedra, a cornercorner with one LiO6 pentagonal pyramid, corners with six VO4 tetrahedra, and edges with two equivalent LiO6 octahedra. The corner-sharing octahedral tilt angles are 58°. There are a spread of Mn–O bond distances ranging from 1.90–1.98 Å. In the third Mn+3.86+ site, Mn+3.86+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six VO4 tetrahedra and faces with two equivalent LiO6 octahedra. There are a spread of Mn–O bond distances ranging from 1.87–1.95 Å. In the fourth Mn+3.86+ site, Mn+3.86+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six VO4 tetrahedra and faces with two equivalent LiO6 octahedra. There are a spread of Mn–O bond distances ranging from 1.88–2.00 Å. In the fifth Mn+3.86+ site, Mn+3.86+ is bonded to six O2- atoms to form MnO6 octahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one LiO6 pentagonal pyramid, corners with six VO4 tetrahedra, and edges with two equivalent LiO6 octahedra. The corner-sharing octahedral tilt angles are 54°. There are a spread of Mn–O bond distances ranging from 1.88–2.09 Å. In the sixth Mn+3.86+ site, Mn+3.86+ is bonded to six O2- atoms to form MnO6 octahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one LiO6 pentagonal pyramid, corners with six VO4 tetrahedra, and edges with two equivalent LiO6 octahedra. The corner-sharing octahedral tilt angles are 54°. There are a spread of Mn–O bond distances ranging from 1.88–2.08 Å. In the seventh Mn+3.86+ site, Mn+3.86+ is bonded to six O2- atoms to form MnO6 octahedra that share a cornercorner with one LiO6 octahedra, a cornercorner with one LiO6 pentagonal pyramid, corners with six VO4 tetrahedra, and edges with two equivalent LiO6 octahedra. The corner-sharing octahedral tilt angles are 56°. There are a spread of Mn–O bond distances ranging from 1.87–1.97 Å. There are forty-eight inequivalent O2- sites. In the first O2- site, O2- is bonded in a trigonal planar geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the second O2- site, O2- is bonded in a trigonal planar geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the third O2- site, O2- is bonded in a trigonal planar geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the fourth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the fifth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the sixth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the seventh O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the eighth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the ninth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the tenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the eleventh O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the twelfth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the thirteenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the fourteenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the fifteenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the sixteenth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the seventeenth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the eighteenth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V5+, and one Mn+3.86+ atom. In the nineteen